#------------------------------------------------------------------------------
#$Date: 2016-03-25 14:53:10 +0200 (Fri, 25 Mar 2016) $
#$Revision: 179904 $
#$URL: svn://www.crystallography.net/cod/cif/7/02/00/7020038.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7020038
loop_
_publ_author_name
'Williams, Edward R.'
'Morris, Samuel A.'
'Weller, Mark T.'
_publ_section_title
;
 Copper(ii) fluorophosphates.
;
_journal_issue                   35
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              10845
_journal_page_last               10853
_journal_paper_doi               10.1039/c2dt31131c
_journal_volume                  41
_journal_year                    2012
_chemical_formula_sum            'Cs Cu2 F3 O6 P2'
_chemical_formula_weight         474.95
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2012-05-11 # Formatted by publCIF
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   9.0219(5)
_cell_length_b                   6.2059(4)
_cell_length_c                   14.3280(7)
_cell_measurement_reflns_used    6763
_cell_measurement_temperature    120(2)
_cell_measurement_theta_max      27.48
_cell_measurement_theta_min      2.91
_cell_volume                     802.21(8)
_computing_cell_refinement
'DENZO (Otwinowski & Minor, 1997) & COLLECT (Hooft, R.W.W., 1998)'
_computing_data_collection       'COLLECT (Hooft, R.W.W., 1998)'
_computing_data_reduction
'DENZO (Otwinowski & Minor, 1997) & COLLECT (Hooft, R.W.W., 1998)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      120(2)
_diffrn_detector_area_resol_mean '4096x4096pixels / 62x62mm'
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type
'Bruker-Nonius APEX II CCD camera on κ-goniostat'
_diffrn_measurement_method       'φ & ω scans'
_diffrn_radiation_monochromator  '10cm confocal mirrors'
_diffrn_radiation_source         'Bruker-Nonius FR591 rotating anode'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0821
_diffrn_reflns_av_sigmaI/netI    0.0561
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            6746
_diffrn_reflns_theta_full        27.52
_diffrn_reflns_theta_max         27.52
_diffrn_reflns_theta_min         3.58
_exptl_absorpt_coefficient_mu    10.226
_exptl_absorpt_correction_T_max  0.7841
_exptl_absorpt_correction_T_min  0.2677
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS 2007/2 (Sheldrick, G.M., 2007)'
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    3.932
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             872
_exptl_crystal_size_max          0.17
_exptl_crystal_size_mid          0.03
_exptl_crystal_size_min          0.03
_refine_diff_density_max         1.586
_refine_diff_density_min         -1.627
_refine_diff_density_rms         0.334
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.166
_refine_ls_matrix_type           full
_refine_ls_number_parameters     82
_refine_ls_number_reflns         1003
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.166
_refine_ls_R_factor_all          0.0935
_refine_ls_R_factor_gt           0.0627
_refine_ls_shift/su_max          0.016
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0000P)²+28.4906P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1091
_refine_ls_wR_factor_ref         0.1244
_reflns_number_gt                753
_reflns_number_total             1003
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            c2dt31131c.txt
_cod_data_source_block           2011erw026_pnma
_cod_original_sg_symbol_H-M      Pnma
_cod_database_code               7020038
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z'
'-x-1/2, y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
O1 O 0.1658(11) 0.0540(14) 0.6153(8) 0.051(3) Uani 1 1 d .
O2 O 0.3696(11) 0.2500 0.5286(8) 0.023(3) Uani 1 2 d S
O3B O -0.430(3) -0.039(4) 0.6280(15) 0.023(2) Uiso 0.390(13) 1 d P
O3A O -0.4885(16) -0.048(2) 0.6346(9) 0.023(2) Uiso 0.610(13) 1 d P
O4A O 0.031(2) -0.2500 0.7161(14) 0.031(4) Uani 0.610(13) 2 d SP
F4B F -0.082(3) -0.2500 0.7626(18) 0.031(4) Uani 0.390(13) 2 d SP
F1 F 0.3023(10) -0.2500 0.5038(7) 0.027(2) Uani 1 2 d S
F5A F -0.269(2) -0.2500 0.6712(14) 0.062(6) Uani 0.610(13) 2 d SP
O5B O 0.192(4) -0.2500 0.744(3) 0.062(6) Uani 0.390(13) 2 d SP
F7 F 0.1136(14) 0.2500 0.4735(9) 0.090(6) Uani 1 2 d S
P4 P 0.2091(5) 0.2500 0.5618(3) 0.0227(9) Uani 1 2 d S
P5 P -0.4378(5) -0.2500 0.6818(3) 0.0207(9) Uani 1 2 d S
Cu2 Cu 0.1856(3) -0.2500 0.61312(15) 0.0319(6) Uani 1 2 d S
Cu3 Cu 0.5000 0.0000 0.5000 0.0217(4) Uani 1 2 d S
Cs1 Cs -0.15274(13) 0.2500 0.69101(8) 0.0326(3) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
P4 O1 Cu2 141.2(6) . .
P4 O1 Cs1 95.5(4) . .
Cu2 O1 Cs1 117.0(4) . .
P4 O1 Cs1 90.1(5) . 6_657
Cu2 O1 Cs1 108.7(5) . 6_657
Cs1 O1 Cs1 91.1(2) . 6_657
P4 O2 Cu3 128.8(2) . 3_656
P4 O2 Cu3 128.8(2) . .
Cu3 O2 Cu3 102.5(4) 3_656 .
O3A O3B P5 77(3) . .
O3A O3B Cu3 82(3) . 1_455
P5 O3B Cu3 124.6(14) . 1_455
O3A O3B Cs1 141(4) . .
P5 O3B Cs1 112.0(11) . .
Cu3 O3B Cs1 116.5(9) 1_455 .
O3A O3B Cs1 53(3) . 6_557
P5 O3B Cs1 92.1(9) . 6_557
Cu3 O3B Cs1 114.7(9) 1_455 6_557
Cs1 O3B Cs1 87.4(5) . 6_557
O3B O3A P5 82(3) . .
O3B O3A Cu3 82(3) . 1_455
P5 O3A Cu3 126.2(9) . 1_455
O3B O3A Cs1 119(3) . 6_557
P5 O3A Cs1 104.7(6) . 6_557
Cu3 O3A Cs1 127.6(6) 1_455 6_557
O3B O3A Cs1 34(3) . .
P5 O3A Cs1 94.1(6) . .
Cu3 O3A Cs1 100.7(5) 1_455 .
Cs1 O3A Cs1 85.6(3) 6_557 .
F4B O4A P5 67.9(15) . 6_657
F4B O4A O5B 131(2) . .
P5 O4A O5B 63.4(16) 6_657 .
F4B O4A Cu2 166.6(18) . .
P5 O4A Cu2 125.6(12) 6_657 .
O5B O4A Cu2 62.1(16) . .
F4B O4A Cs1 70.3(6) . 1_545
P5 O4A Cs1 100.9(5) 6_657 1_545
O5B O4A Cs1 118.6(3) . 1_545
Cu2 O4A Cs1 104.4(4) . 1_545
F4B O4A Cs1 70.3(6) . .
P5 O4A Cs1 100.9(5) 6_657 .
O5B O4A Cs1 118.6(3) . .
Cu2 O4A Cs1 104.4(4) . .
Cs1 O4A Cs1 122.7(6) 1_545 .
O4A F4B P5 64.6(15) . 6_657
O4A F4B Cs1 89.5(7) . 1_545
P5 F4B Cs1 108.9(5) 6_657 1_545
O4A F4B Cs1 89.5(7) . .
P5 F4B Cs1 108.9(5) 6_657 .
Cs1 F4B Cs1 137.5(8) 1_545 .
Cu2 F1 Cu3 116.1(4) . .
Cu2 F1 Cu3 116.1(4) . 3_646
Cu3 F1 Cu3 82.0(3) . 3_646
Cu2 F1 Cs1 120.3(4) . 5_556
Cu3 F1 Cs1 107.9(3) . 5_556
Cu3 F1 Cs1 107.9(3) 3_646 5_556
O5B F5A P5 68.2(17) 6_557 .
O5B F5A Cs1 90.3(7) 6_557 .
P5 F5A Cs1 108.0(3) . .
O5B F5A Cs1 90.3(7) 6_557 1_545
P5 F5A Cs1 108.0(3) . 1_545
Cs1 F5A Cs1 141.3(7) . 1_545
F5A O5B O4A 122(3) 6_657 .
F5A O5B P5 64.0(18) 6_657 6_657
O4A O5B P5 57.6(14) . 6_657
F5A O5B Cu2 166(3) 6_657 .
O4A O5B Cu2 72.7(19) . .
P5 O5B Cu2 130(2) 6_657 .
F5A O5B Cs1 68.8(9) 6_657 6_657
O4A O5B Cs1 116.9(6) . 6_657
P5 O5B Cs1 96.8(9) 6_657 6_657
Cu2 O5B Cs1 105.9(7) . 6_657
F5A O5B Cs1 68.8(9) 6_657 6_647
O4A O5B Cs1 116.9(6) . 6_647
P5 O5B Cs1 96.8(9) 6_657 6_647
Cu2 O5B Cs1 105.9(7) . 6_647
Cs1 O5B Cs1 123.2(12) 6_657 6_647
O1 P4 O1 109.4(7) 7_565 .
O1 P4 O2 114.2(5) 7_565 .
O1 P4 O2 114.2(5) . .
O1 P4 F7 106.1(6) 7_565 .
O1 P4 F7 106.1(6) . .
O2 P4 F7 106.1(7) . .
O1 P4 Cs1 61.2(4) 7_565 .
O1 P4 Cs1 61.2(4) . .
O2 P4 Cs1 168.6(5) . .
F7 P4 Cs1 85.3(5) . .
O1 P4 Cs1 66.5(5) 7_565 6_657
O1 P4 Cs1 66.5(5) . 6_657
O2 P4 Cs1 88.8(5) . 6_657
F7 P4 Cs1 165.1(5) . 6_657
Cs1 P4 Cs1 79.83(8) . 6_657
O4A P5 O3A 112.7(7) 6_557 7
O4A P5 O3A 112.7(7) 6_557 .
O3A P5 O3A 113.8(11) 7 .
O4A P5 O3B 120.4(8) 6_557 .
O3A P5 O3B 120.4(8) 7 .
O3A P5 O3B 20.6(9) . .
O4A P5 O3B 120.4(9) 6_557 7
O3A P5 O3B 20.6(9) 7 7
O3A P5 O3B 120.4(8) . 7
O3B P5 O3B 118.8(17) . 7
O4A P5 F5A 106.7(11) 6_557 .
O3A P5 F5A 105.0(7) 7 .
O3A P5 F5A 105.0(7) . .
O3B P5 F5A 84.4(10) . .
O3B P5 F5A 84.4(10) 7 .
O4A P5 F4B 47.6(12) 6_557 6_557
O3A P5 F4B 88.5(8) 7 6_557
O3A P5 F4B 88.5(8) . 6_557
O3B P5 F4B 107.7(10) . 6_557
O3B P5 F4B 107.7(10) 7 6_557
F5A P5 F4B 154.3(13) . 6_557
O4A P5 O5B 58.9(17) 6_557 6_557
O3A P5 O5B 122.0(6) 7 6_557
O3A P5 O5B 122.0(6) . 6_557
O3B P5 O5B 107.8(11) . 6_557
O3B P5 O5B 107.8(11) 7 6_557
F5A P5 O5B 47.8(16) . 6_557
F4B P5 O5B 106.5(19) 6_557 6_557
O4A P5 Cs1 95.1(5) 6_557 .
O3A P5 Cs1 148.7(6) 7 .
O3A P5 Cs1 64.2(6) . .
O3B P5 Cs1 47.5(9) . .
O3B P5 Cs1 130.5(9) 7 .
F5A P5 Cs1 50.85(11) . .
F4B P5 Cs1 121.8(5) 6_557 .
O5B P5 Cs1 60.3(7) 6_557 .
O4A P5 Cs1 95.1(5) 6_557 1_545
O3A P5 Cs1 64.2(6) 7 1_545
O3A P5 Cs1 148.7(6) . 1_545
O3B P5 Cs1 130.5(9) . 1_545
O3B P5 Cs1 47.5(9) 7 1_545
F5A P5 Cs1 50.85(11) . 1_545
F4B P5 Cs1 121.8(4) 6_557 1_545
O5B P5 Cs1 60.3(7) 6_557 1_545
Cs1 P5 Cs1 100.62(10) . 1_545
O4A P5 Cs1 58.1(4) 6_557 6_547
O3A P5 Cs1 54.6(5) 7 6_547
O3A P5 Cs1 133.8(6) . 6_547
O3B P5 Cs1 154.3(9) . 6_547
O3B P5 Cs1 66.1(9) 7 6_547
F5A P5 Cs1 121.1(4) . 6_547
F4B P5 Cs1 50.42(19) 6_557 6_547
O5B P5 Cs1 93.1(10) 6_557 6_547
Cs1 P5 Cs1 150.72(11) . 6_547
Cs1 P5 Cs1 72.78(2) 1_545 6_547
O4A P5 Cs1 58.1(4) 6_557 6_557
O3A P5 Cs1 133.8(6) 7 6_557
O3A P5 Cs1 54.6(5) . 6_557
O3B P5 Cs1 66.1(9) . 6_557
O3B P5 Cs1 154.3(9) 7 6_557
F5A P5 Cs1 121.1(4) . 6_557
F4B P5 Cs1 50.42(19) 6_557 6_557
O5B P5 Cs1 93.1(10) 6_557 6_557
Cs1 P5 Cs1 72.78(2) . 6_557
Cs1 P5 Cs1 150.72(11) 1_545 6_557
Cs1 P5 Cs1 98.77(9) 6_547 6_557
O5B Cu2 F1 144.3(11) . .
O5B Cu2 O1 89.2(4) . .
F1 Cu2 O1 93.8(3) . .
O5B Cu2 O1 89.2(4) . 7
F1 Cu2 O1 93.8(3) . 7
O1 Cu2 O1 169.0(6) . 7
O5B Cu2 O4A 45.2(12) . .
F1 Cu2 O4A 170.5(6) . .
O1 Cu2 O4A 85.6(3) . .
O1 Cu2 O4A 85.6(3) 7 .
O5B Cu2 Cs1 177.9(11) . 5_556
F1 Cu2 Cs1 37.8(3) . 5_556
O1 Cu2 Cs1 90.6(4) . 5_556
O1 Cu2 Cs1 90.6(4) 7 5_556
O4A Cu2 Cs1 132.7(5) . 5_556
O3B Cu3 O3B 180.000(3) 1_655 5_556
O3B Cu3 O3A 15.9(7) 1_655 1_655
O3B Cu3 O3A 164.1(7) 5_556 1_655
O3B Cu3 O3A 164.1(7) 1_655 5_556
O3B Cu3 O3A 15.9(7) 5_556 5_556
O3A Cu3 O3A 180.000(1) 1_655 5_556
O3B Cu3 O2 95.4(8) 1_655 .
O3B Cu3 O2 84.6(8) 5_556 .
O3A Cu3 O2 87.0(5) 1_655 .
O3A Cu3 O2 93.0(5) 5_556 .
O3B Cu3 O2 84.6(8) 1_655 5_656
O3B Cu3 O2 95.4(8) 5_556 5_656
O3A Cu3 O2 93.0(5) 1_655 5_656
O3A Cu3 O2 87.0(5) 5_556 5_656
O2 Cu3 O2 180.000(1) . 5_656
O3B Cu3 F1 81.9(7) 1_655 5_656
O3B Cu3 F1 98.1(7) 5_556 5_656
O3A Cu3 F1 94.8(5) 1_655 5_656
O3A Cu3 F1 85.2(5) 5_556 5_656
O2 Cu3 F1 86.5(3) . 5_656
O2 Cu3 F1 93.5(3) 5_656 5_656
O3B Cu3 F1 98.1(7) 1_655 .
O3B Cu3 F1 81.9(7) 5_556 .
O3A Cu3 F1 85.2(5) 1_655 .
O3A Cu3 F1 94.8(5) 5_556 .
O2 Cu3 F1 93.5(3) . .
O2 Cu3 F1 86.5(3) 5_656 .
F1 Cu3 F1 180.0(3) 5_656 .
F1 Cs1 O3B 53.7(4) 5_556 .
F1 Cs1 O3B 53.7(4) 5_556 7_565
O3B Cs1 O3B 68.0(8) . 7_565
F1 Cs1 F5A 77.5(4) 5_556 .
O3B Cs1 F5A 36.7(5) . .
O3B Cs1 F5A 104.7(5) 7_565 .
F1 Cs1 F5A 77.5(4) 5_556 1_565
O3B Cs1 F5A 104.7(5) . 1_565
O3B Cs1 F5A 36.7(5) 7_565 1_565
F5A Cs1 F5A 141.3(7) . 1_565
F1 Cs1 O1 94.8(3) 5_556 7_565
O3B Cs1 O1 142.4(5) . 7_565
O3B Cs1 O1 112.3(5) 7_565 7_565
F5A Cs1 O1 126.7(3) . 7_565
F5A Cs1 O1 84.4(3) 1_565 7_565
F1 Cs1 O1 94.8(3) 5_556 .
O3B Cs1 O1 112.3(4) . .
O3B Cs1 O1 142.4(5) 7_565 .
F5A Cs1 O1 84.4(3) . .
F5A Cs1 O1 126.7(3) 1_565 .
O1 Cs1 O1 43.2(3) 7_565 .
F1 Cs1 F4B 111.1(4) 5_556 1_565
O3B Cs1 F4B 139.2(6) . 1_565
O3B Cs1 F4B 73.4(6) 7_565 1_565
F5A Cs1 F4B 165.2(6) . 1_565
F5A Cs1 F4B 37.7(5) 1_565 1_565
O1 Cs1 F4B 65.9(5) 7_565 1_565
O1 Cs1 F4B 106.2(5) . 1_565
F1 Cs1 F4B 111.1(4) 5_556 .
O3B Cs1 F4B 73.4(6) . .
O3B Cs1 F4B 139.2(6) 7_565 .
F5A Cs1 F4B 37.7(5) . .
F5A Cs1 F4B 165.2(6) 1_565 .
O1 Cs1 F4B 106.2(5) 7_565 .
O1 Cs1 F4B 65.9(5) . .
F4B Cs1 F4B 137.5(8) 1_565 .
F1 Cs1 O1 121.2(2) 5_556 4_456
O3B Cs1 O1 93.1(4) . 4_456
O3B Cs1 O1 70.0(4) 7_565 4_456
F5A Cs1 O1 104.5(3) . 4_456
F5A Cs1 O1 65.4(3) 1_565 4_456
O1 Cs1 O1 123.2(3) 7_565 4_456
O1 Cs1 O1 143.9(2) . 4_456
F4B Cs1 O1 60.9(5) 1_565 4_456
F4B Cs1 O1 99.9(5) . 4_456
F1 Cs1 O1 121.2(2) 5_556 6_557
O3B Cs1 O1 70.0(4) . 6_557
O3B Cs1 O1 93.1(4) 7_565 6_557
F5A Cs1 O1 65.4(3) . 6_557
F5A Cs1 O1 104.5(3) 1_565 6_557
O1 Cs1 O1 143.9(2) 7_565 6_557
O1 Cs1 O1 123.2(3) . 6_557
F4B Cs1 O1 99.9(5) 1_565 6_557
F4B Cs1 O1 60.9(5) . 6_557
O1 Cs1 O1 41.4(3) 4_456 6_557
F1 Cs1 O3A 147.2(2) 5_556 4_556
O3B Cs1 O3A 147.2(5) . 4_556
O3B Cs1 O3A 103.8(4) 7_565 4_556
F5A Cs1 O3A 135.0(4) . 4_556
F5A Cs1 O3A 72.1(4) 1_565 4_556
O1 Cs1 O3A 70.5(3) 7_565 4_556
O1 Cs1 O3A 93.5(3) . 4_556
F4B Cs1 O3A 36.3(5) 1_565 4_556
F4B Cs1 O3A 101.3(5) . 4_556
O1 Cs1 O3A 55.3(3) 4_456 4_556
O1 Cs1 O3A 79.0(3) 6_557 4_556
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
O1 P4 1.490(9) .
O1 Cu2 1.895(9) .
O1 Cs1 3.304(9) .
O1 Cs1 3.444(12) 6_657
O2 P4 1.524(10) .
O2 Cu3 1.990(6) 3_656
O2 Cu3 1.990(6) .
O3B O3A 0.54(2) .
O3B P5 1.52(2) .
O3B Cu3 1.96(2) 1_455
O3B Cs1 3.21(2) .
O3B Cs1 3.74(2) 6_557
O3A P5 1.494(14) .
O3A Cu3 1.955(13) 1_455
O3A Cs1 3.444(14) 6_557
O3A Cs1 3.641(15) .
O4A F4B 1.22(3) .
O4A P5 1.490(19) 6_657
O4A O5B 1.51(4) .
O4A Cu2 2.03(2) .
O4A Cs1 3.535(9) 1_545
O4A Cs1 3.535(9) .
F4B P5 1.53(2) 6_657
F4B Cs1 3.329(9) 1_545
F4B Cs1 3.329(9) .
F1 Cu2 1.887(9) .
F1 Cu3 2.365(7) .
F1 Cu3 2.365(7) 3_646
F1 Cs1 3.100(10) 5_556
F5A O5B 1.26(4) 6_557
F5A P5 1.527(19) .
F5A Cs1 3.289(7) .
F5A Cs1 3.289(7) 1_545
O5B F5A 1.26(4) 6_657
O5B P5 1.58(3) 6_657
O5B Cu2 1.88(4) .
O5B Cs1 3.53(2) 6_657
O5B Cs1 3.53(2) 6_647
F7 P4 1.531(14) .
P4 O1 1.490(9) 7_565
P4 Cs1 3.753(4) .
P4 Cs1 3.754(5) 6_657
P5 O4A 1.490(19) 6_557
P5 O3A 1.494(14) 7
P5 O3B 1.52(2) 7
P5 F4B 1.53(2) 6_557
P5 O5B 1.58(3) 6_557
P5 Cs1 4.032(3) .
P5 Cs1 4.032(3) 1_545
P5 Cs1 4.088(3) 6_547
P5 Cs1 4.088(3) 6_557
Cu2 O1 1.895(9) 7
Cu2 Cs1 4.368(2) 5_556
Cu3 O3B 1.96(2) 1_655
Cu3 O3B 1.96(2) 5_556
Cu3 O3A 1.955(13) 1_655
Cu3 O3A 1.955(13) 5_556
Cu3 O2 1.990(6) 5_656
Cu3 F1 2.365(7) 5_656
Cs1 F1 3.100(10) 5_556
Cs1 O3B 3.21(2) 7_565
Cs1 F5A 3.289(7) 1_565
Cs1 O1 3.304(9) 7_565
Cs1 F4B 3.329(9) 1_565
Cs1 O1 3.444(12) 4_456
Cs1 O1 3.444(12) 6_557
Cs1 O3A 3.444(14) 4_556
